TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS


 Barry Lambert
 1 years ago
 Views:
Transcription
1 TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering and Applied Science, Northwestern University 37 Sheridan Road, Evanston, IL 68 USA Research Assistant, Theoretical and Applied Mechanics, Robert R. McCormick School of Engineering and Applied Science, Northwestern University, 37 Sheridan Road, Evanston, IL 68 USA SUMMARY: The objective of this work was to study the behavior of composite sandwich structures and develop simple models to explain this behavior as a function of material, geometric and loading parameters. The scope of the study consists of mechanical characterization of the sandwich constituent materials, i.e., composite facings, honeycomb and foam cores, and adhesive layers; fabrication and testing of sandwich beams in bending; identification and recording of failure mechanisms by direct observation and nondestructive evaluation; and comparison of observed deformation and failure behavior with analytical predictions. The beam facings displayed the characteristic nonlinearities of the composite material used, a softening nonlinearity on the compression side and a stiffening one of the tension side. The linear response of the beam is perfectly described by a simple bending model neglecting the contribution of the core, however, the more pronounced nonlinear behavior requires more accurate characterization of the core and adhesive materials separately, and more refined modeling. KEYWORDS: Sandwich beams, fabrication, carbon/epoxy composite, honeycomb cores, foam cores, test methods, modeling, nonlinear response, failure mechanisms. INTRODUCTION Sandwich construction is of particular interest and widely used in many structures, because the concept is very suitable and amenable to the development of lightweight structures with high inplane and flexural stiffness. Sandwich panels consist typically of two thin face sheets or facings or skins and a lightweight thicker core. Commonly used materials for facings are composite laminates and metals, while cores are made of metallic and nonmetallic honeycombs, cellular foams, balsa wood or trusses. The face sheets are typically bonded to the core with adhesive. The facings carry most of the bending and in plane loads and the core defines the flexural stiffness and outofplane shear and compressive behavior. The structural
2 performance of sandwich panels depends not only on the properties of the skins, but also on those of the core and the adhesive bonding the core to the skins, as well as on the geometrical dimensions of the components. Important issues in sandwich structures are the quality of the structure, the various failure mechanisms that are developed under various loading conditions, effects of nonlinear material behavior and effects of geometric nonlinearities. A great deal of work has been published on the behavior of sandwich structures in the last few decades. Many analytical and computational models are available to describe the behavior of sandwich beams, panels and shells under different loading conditions. The fundamentals of sandwich construction and reviews of analytical and computational methods are described in recent works by Zenkert [], Noor et al. [] and Reddy [3]. Many of the models proposed to date are approximations to the threedimensional elasticity theory based on assumptions for the displacements, strains and/or stresses through the thickness. The validity of the various approximations depends on the geometry of the beam, properties of the component materials and loading conditions. Most theories assume linear elastic behavior for the component materials and small deflections. However, material and geometric nonlinearities are important issues. In addition to modeling material behavior, the relative motions of the facings must be taken into account in the socalled multilayer buildup theory [,5]. When transverse deflections become of the order of the beam depth nonlinear analyses may be necessary [6]. Several papers have discussed the nonlinear load deflection behavior of sandwich plates [79]. The objective of this work is to study experimentally the behavior of composite sandwich beams under pure bending and threepoint bending and compare the results with predictions of theoretical models. EXPERIMENTAL PROCEDURE The sandwich beam facings were unidirectional carbon/epoxy plates (AS/356). The facing plates as well as additional plates for material characterization were fabricated by autoclave molding. Uniaxial tensile and compressive tests were conducted primarily in the longitudinal direction in order to obtain the relevant constitutive behavior of the facing material. The longitudinal tensile and compressive stressstrain behavior for the AS/356 carbon/epoxy is shown in Fig.. It can be seen that the material exhibits a characteristic stiffening nonlinearity in tension and softening nonlinearity in compression. One of the core materials used in this study was aluminum honeycomb PAMG 8.3/6 P55 (Plascore Co., 55 aluminum alloy, 8. lb/ft 3 density, 3/6 in. cell size,. in. foil gauge). The material is highly anisotropic. The inplane stiffnesses E and E and the outofplane stiffness E 3 (along the cell axis) were obtained by means of flexural and pure compression tests. The outofplane shear modulus was obtained by means of a railshear test. The second core material used was a PVC closedcell foam (Divinycell H). The material was tested under tension, compression and shear. The adhesive used to bond the facings to the honeycomb core was FM73M film adhesive (CytecFiberite). It is a.5 mm (. in.) thick toughened epoxy layer reinforced with glass fabric. The shear properties of the adhesive were determined by using the Arcan fixture. Some characteristic properties of the sandwich component materials are tabulated in Table. The honeycomb core was.5 cm ( in.) wide and was machined from the.5 cm ( in.) thick sheet along the stiffer (E ) direction. The.5 cm ( in.) wide composite facings were machined from the unidirectional plates, bonded to the top and bottom faces of the honeycomb
3 core with FM73 M film adhesive and the assembly was cured under pressure in an oven following the recommended curing cycle for the adhesive. Sandwich beams were also prepared by bonding composite facings to foam cores of.5 x.5 cm ( x in.) cross section using a commercially available epoxy adhesive (Hysol EA 93). σ Tension σ.5.5 Strain, ε (%) Fig. : Longitudinal tensile and compressive stressstrain behavior of AS/356 unidirectional carbon/epoxy. Table : Characteristic Properties of Sandwich Constituent Materials Honeycomb FM73Foam Facing Core Adhesive Core Density, ρ, kg/m 3 (lb / ft 3 ),6 () 9 (8.),8 (7) (6.) Thickness, h, mm (in.). (.) 5. (.).5 (.) 5. (.) Longitudinal Modulus, 7, (,6) 8.7 (.),7 (7) (7.5) E, MPa (ksi) Transverse Shear Modulus, 7,6 (,) 58 (8) (6) 8 (6.9) G 3, MPa (ksi) Transverse Shear Strength, ~ 7 (.3).6 (.38) 33 (.8).6 (.3) F 3, MPa (ksi) Beams for fourpoint flexural testing were 5.7 cm (8 in.) long. Because of the low shear strength of the core, shear damage occurred early in the core near the points of load application. In order to prevent premature failures under the loads and to insure failure in the pure bending section, the outer core sections subjected to shear were reinforced by filling the cells with epoxy. Better results were obtained when this cell reinforcement was tapered off gradually into the pure bending section. Strains on the outer surfaces of the facings as well as on the inner surfaces, at the interface with the adhesive bond, were recorded with strain gages. Most of the gages were oriented along the axis of the beam, but some were mounted in the transverse direction to record transverse strains. The deflection of the beams was measured with a displacement transducer (LVDT) and also monitored with a coarse moiré grating (3 lines/cm, 8 lines/in.). The displacement
4 field in the core was recorded with a finer moiré grating of 8 lines/cm (3 lines/in.). Before applying the moiré gratings, the lateral surface of the core was coated with a white silicone rubber layer to make the surface smooth and reflective. Sandwich beams were loaded under fourpoint and threepoint flexure in a servohydraulic machine, while recording load, strain gage, moiré and LVDT data. All specimens were loaded to failure. The fourpoint bending tests produced compressive facing failures at strains of over.5%. The threepoint bending tests were carried out until core failure occurred. Beams under FourPoint Bending RESULTS The applied bending moment was plotted versus the outer surface longitudinal strains for a beam with honeycomb core under fourpoint bending in Fig.. The same type of stiffening and softening nonlinearities observed before for the facing materials are seen here. Failure was governed by the compressive strength of the facing, which in this case reached a value of 93 MPa (8 ksi), higher than any recorded value for this material under direct compression. The ultimate compressive strain recorded was.6% Tension Strain, ε (%) Fig : Applied moment versus longitudinal strains for sandwich beam with honeycomb core under fourpoint bending. Before comparing the experimental results with available models, the variation of the longitudinal strain through the facing thickness was investigated. Results from another test in Figs. 3 and show the variation with applied moment of longitudinal strains on the outer and inner surfaces of the facings. It is seen that these strains are not constant through the thickness of the facing. Analysis of the data indicates that the inner surface strains are between 3.5 and.% lower (in absolute terms) than the corresponding outer surface strains. A linear strain variation through the entire beam section would imply strain differences of %.
5 .5.5 Outer Strain Inner Strain Tension Strain, ε (%) Fig. 3: Applied moment versus longitudinal strains on surfaces of tension facing of sandwich beam under fourpoint bending..5.5 Outer Strain Inner Strain Strain, ε (%) Fig. : Applied moment versus longitudinal strains on surfaces of compression facing of sandwich beam under fourpoint bending. The strain field in the core was investigated by the moiré technique discussed before. A moiré fringe pattern corresponding to longitudinal displacements in the core is shown in Fig. 5. A linear strain variation through the thickness in the pure bending zone would imply the following form for the strain and displacement ε ( z) = cz = u () x u x, z ( ) = cxz ()
6 since u (,z) = (along vertical axis of symmetry) The moiré fringes, being loci of equal displacements, do indeed have the form of hyperbolas and are equidistant along any horizontal line. Furthermore, there is evidence that the neutral axis has shifted toward the tension side because of the different nonlinearities of the tension and compression facings. Fig. 5: Moire fringe pattern in the core corresponding to longitudinal displacements ( lines/mm; 3 lines/in.) Beams under ThreePoint Bending Under threepoint bending and without any special core reinforcement, all beams (with honeycomb core) failed early due to shear crimping of the core. The failure load, being twice the shear force, remained nearly constant for varying span lengths. This means that as the span length decreases, the applied maximum moment, and thereby the maximum facing strains, at failure decrease (Fig. 6). The results also indicate that even in cases of increased shear loading of the core, the bending moment is carried almost entirely by the facings. Beams with foam cores were tested under threepoint bending and strains and deflections were recorded. Figure 7 shows loaddeflection curves for two cases. In the cases recorded, where the facing sheets were 8 plies and plies thick (mm and.5mm thick, respectively) the beams failed by local indentation and crushing of the core under the applied load. In this case, failure is not governed by the shear strength of the core, but by a combination of flexural stiffness of the facing and compressive strength of the core. A finite element analysis is in progress to evaluate the behavior of such beams as a function of material and geometric parameters. Modeling The objective of the modeling was to predict the relationship between applied loading (moment) and stresses or strains in the sandwich beams, based on the properties and dimensions of the components of the beam. Referring to the schematic of a sandwich beam in Fig. 8, the neutral axis is located at a distance. e = E fc h f d + E c h c ( h c + h f )/ (3) ( E ft + E fc )h f + E c h c and for a weak core, E c << E ft, E fc,
7 .5..3 L=8" L=" L=" Tension L L Strain, ε (%) Fig. 6: Applied moment versus maximum facing strain for beams of different span length under threepoint bending. 5 8 plies plies 5 5 Deflection (mm) Fig. 7: Applied load versus deflection for beams with foam cores and two facing thicknesses. M z E fc M h f h c z Neutral axis E c Eft x y e h f Fig. 8: Schematic of sandwich beam.
8 (5) e where d = h c + h f The bending stiffness for a weak core is D = h 3 f E fc d () ( E ft + E fc )h f ( E ft + E fc ) + E ft E fc h f d E ft + E fc For thin facings, h f << h c we have E D ft E fc h f d (6) E ft + E fc The normal stresses in the facings and core are ( ) = Mz σ ft, σ fc, σ c D ( ) (7) E ft, E fc, E c For a weak core and thin facings σ ft = σ fc where b = width of beam M db h f The experimentally obtained stressstrain relationships of the facing material in tension and compression and that of the honeycomb core were used to obtain momentstrain relations. Different cases/assumptions were considered in modeling the sandwich beams tested under pure bending. The first case where a linear variation of strain through the thickness is assumed with a neutral axis through the centroid of the cross section is only valid in the linear range of the facing material. At higher loads, the nonlinear response of the facings must be considered, although other simplifying assumptions can be made. For example, the core contribution could be neglected since its modulus is much smaller than the facing modulus (E c << E f ). The strain, and hence the stress, in the facings can be assumed to vary linearly or to be constant through the facing thickness. The latter assumption is valid when the facing thickness is much smaller than the core thickness (h f << h c ). In the present case two models were implemented, one by assuming linear variation of strain through the facing thickness and the other by assuming a constant strain through the facing thickness. In both models the core contribution was neglected. The nonlinear behavior of the facing material was considered in an incremental computational scheme. Results are plotted in Fig. 9 and compared with experimental momentstrain results. It appears that the assumption of constant strain gives better agreement with experimental results. The agreement is satisfactory in general. The small discrepancies observed are not attributed to the model but rather to the difficulty in obtaining reliable stressstrain curves in direct longitudinal compression. The contribution of the core to the momentstrain relations was found to be negligible. The effect of core modulus was investigated using a model with the assumption of constant strain through the facing thickness. Results are shown in Fig. for the compression and facing. Similar results were obtained for the tension facing. It appears that the influence of the core is not noticeable until its stiffness is approximately / times the facing modulus.
9 .5.5 Experimental Model (Linear Strain) Model (Constant Strain) Tension.5.5 Strain, ε (%) Fig. 9: Experimental and predicted momentstrain curves for two facings of composite sandwich beam under fourpoint bending. Moment (knm),6,,,8,6,, E c = ksi E c =5 ksi E c = ksi E c = ksi 8 E c = ksi Moment (kipin),5,5 Strain, ε (%) Fig. : Effect of core modulus on the momentstrain relationship for sandwich beam under fourpoint bending (compression facing). SUMMARY AND CONCLUSIONS An experimental study was conducted on the behavior of composite sandwich beams under fourpoint and threepoint bending. The sandwich beams were prepared with unidirectional carbon/epoxy facings and aluminum honeycomb or foam cores. Strains in the facings and the core were measured with strain gages and moiré gratings, respectively. The bending behavior of the beams, whether loaded under fourpoint or threepoint bending, is governed by the facings. Therefore, the momentstrain relations for the facings display the same type of nonlinear behavior as the composite material itself, i.e., a stiffening nonlinearity in tension and a softening nonlinearity in compression. A linear variation in strain through the thickness was determined in both core and skins. The contribution of the most widely used cores to the
10 bending stiffness can be neglected. In the case of pure bending, failure takes place on the compressive facing of the beam where the ultimate compressive stress and strain can reach values higher than any recorded for the composite material under direct compression. When shear is present, failure of the honeycomb sandwich beam is governed by the low shear strength of the core, 5 kpa (35 psi) for the honeycomb core used here. In the case of beams with foam cores, indentation failures under the load are common and are controlled by the flexural stiffness of the facing and compressive strength of the core. Experimental results were in good agreement with predictions of simple models assuming the facings to behave like membranes and neglecting the contribution of the core, but accounting for the nonlinear behavior of the facings. ACKNOWLEDGEMENT The work described here was supported by the Office of Naval Research (ONR). The authors would like to thank Dr. Y. D. S. Rajapakse of ONR for his support and cooperation and Mrs. Yolande Mallian for typing the manuscript. REFERENCES. Zenkert, D., "An Introduction to Sandwich Construction," Engineering Materials Advisory Services, London, Noor, A. K., Burton, W. S. and Bert, C. W. Computational Models for Sandwich Panels and Shells, Applied Mechanics Reviews, Vol. 9, 996, pp Reddy, J. N., "Mechanics of Laminated Composite Plates: Theory and Analysis," CRC Press, Boca Raton, FL., Sun, C. T., Microstructure Theory for a Composite Beam, J. of Appl. Mech., Vol. 38, No., 97, pp Kemmochi, K. and Uemura, M., Measurement of Stress Distribution in Sandwich Beams under FourPoint Bending, Exper. Mech., Vol., 98, pp Reissner, E. Finite Deflections of Sandwich Plates, J. Aeronaut. Scie., Vol. 5, 98, pp MeyerPiening., H.R., Remarks on Higher Order Sandwich Stress and Deflection Analysis, Proc. of the First Int. Conf. on Sandwich Constructions, ed. K.A. Olsson & R. P. Reichard. EMAS. West Midlands, UK, 989, pp Reichard, R. P., The Design of FRP Sandwich Panels for Ship and Boat Hulls, in Proc. of the First Int. Conf. on Sandwich Constructions, ed. K.A. Olsson & R. P. Reichard. EMAS. West Midlands, UK, 989, pp BauMadsen, N. K., Svendsen, K.H. and Kildegaard, A. Large Deflections of Sandwich Plates  An Experimental Investigation, Composite Structures, Vol. 3, 993, pp. 75.
Failure modes of composite sandwich beams
Theoret. Appl. Mech., Vol.35, No.13, pp. 105 118, Belgrade 2008 Failure modes of composite sandwich beams E.E. Gdoutos I.M. Daniel Abstract A thorough investigation of failure behavior of composite sandwich
More informationNONLINEAR BEHAVIOUR OF FOAM CORED CURVED SANDWICH PANELS SUBJECTED TO THERMO MECHANICAL LOADING
Included in ONR sessions organized by Yapa D.S. Rajapakse NONLINEAR BEHAVIOUR OF FOAM CORED CURVED SANDWICH PANELS SUBJECTED TO THERMO MECHANICAL LOADING O. T. Thomsen 1) and Y. Frostig 2) 1) Department
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationGEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE
GEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE Prof. J. N. Mandal Department of Civil Engineering, IIT Bombay, Powai, Mumbai 400076, India. Tel.02225767328 email: cejnm@civil.iitb.ac.in Module13 LECTURE
More informationIndentation Energy in Bending of Sandwich Beams with Composite Laminated Faces and Foam Core
Indentation Energy in Bending of Sandwich Beams with Composite Laminated Faces and Foam Core M. SADIGHI, H. POURIAYEVALI, and M. SAADATI Dept. of Mechanical Engineering, Amirkabir University of Tech, Tehran,
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationMECHANICS OF MATERIALS Sample Problem 4.2
Sample Problem 4. SOLUTON: Based on the cross section geometry, calculate the location of the section centroid and moment of inertia. ya ( + Y Ad ) A A castiron machine part is acted upon by a knm couple.
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More informationHomework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. Fall 2004
Homework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. 1. A beam is loaded as shown. The dimensions of the cross section appear in the insert. the figure. Draw a complete free body diagram showing an equivalent
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationInternational Journal for Ignited Minds (IJIMIINDS) Design and Analysis of Effect of Core Thickness in UAV Wing
International Journal for Ignited Minds (IJIMIINDS) Design and Analysis of Effect of Core Thickness in UAV Wing Puttappa H R 1, Ravi Prakash M 2 & Madhusudhan Reddy 3 1 P G Scholar, Dept of Mechanical
More informationProject PAJ2 Dynamic Performance of Adhesively Bonded Joints. Report No. 3 August Proposed Draft for the Revision of ISO
NPL Report CMMT(A)81 Project PAJ2 Dynamic Performance of Adhesively Bonded Joints Report No. 3 August 1997 Proposed Draft for the Revision of ISO 110032 Adhesives  Determination of Shear Behaviour of
More informationPHYSICAL AGING AND CREEP CHARACTERIZATION OF A CARBON/POLYIMIDE COMPOSITE
PHYSICAL AGING AND CREEP CHARACTERIZATION OF A CARBON/POLYIMIDE COMPOSITE I. M. Daniel 1, J. J. Luo 2, and Z. Sun 3 1 Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationStrain Measurement. Prof. Yu Qiao. Department of Structural Engineering, UCSD. Strain Measurement
Strain Measurement Prof. Yu Qiao Department of Structural Engineering, UCSD Strain Measurement The design of loadcarrying components for machines and structures requires information about the distribution
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationSIZE EFFECTS IN THE COMPRESSIVE CRUSHING OF HONEYCOMBS
43rd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Con 2225 April 2002, Denver, Colorado SIZE EFFECTS IN THE COMPRESSIVE CRUSHING OF HONEYCOMBS Erik C. Mellquistand Anthony M.
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 922 from Hibbeler  Statics and Mechanics of Materials) A short
More informationFlexural properties of polymers
A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON
More informationModeling the elastic properties of paper honeycomb panels using the finite element method
Proceedings of the XXVI th International Conference Research for Furniture Industry Modeling the elastic properties of paper honeycomb panels using the finite element method Viktor UTASSY, Levente DÉNES
More informationSamantha Ramirez, MSE
Samantha Ramirez, MSE Centroids The centroid of an area refers to the point that defines the geometric center for the area. In cases where the area has an axis of symmetry, the centroid will lie along
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationIntroduction to Structural Member Properties
Introduction to Structural Member Properties Structural Member Properties Moment of Inertia (I): a mathematical property of a crosssection (measured in inches 4 or in 4 ) that gives important information
More informationSCALING EFFECTS IN THE LOW VELOCITY IMPACT RESPONSE OF FIBRE METAL
SCALING EFFECTS IN THE LOW VELOCITY IMPACT RESPONSE OF FIBRE METAL LAMINATES J. G. Carrillo 1, S. McKown 1, M. Mujib 1 and W. J. Cantwell 1. R. Day 2 1 Department of Engineering, University of Liverpool,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationThis procedure covers the determination of the moment of inertia about the neutral axis.
327 Sample Problems Problem 16.1 The moment of inertia about the neutral axis for the Tbeam shown is most nearly (A) 36 in 4 (C) 236 in 4 (B) 136 in 4 (D) 736 in 4 This procedure covers the determination
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationExperiment Five (5) Principal of Stress and Strain
Experiment Five (5) Principal of Stress and Strain Introduction Objective: To determine principal stresses and strains in a beam made of aluminum and loaded as a cantilever, and compare them with theoretical
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationEffects of Core Softness and Bimodularity of Fibreglass Layers on Flexural Stiffness of Polymer Sandwich Structures
Effects of Core Softness and Bimodularity of Fibreglass Layers on Flexural Stiffness of Polymer Sandwich Structures Oldřich Šuba 1,*, Oldřich Šuba jr. 1, and Soňa Rusnáková 1 1 Tomas Bata University in
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationPOSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS
POSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS  Technical Paper  Tidarut JIRAWATTANASOMKUL *1, Dawei ZHANG *2 and Tamon UEDA *3 ABSTRACT The objective of this study is to propose a new
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationEFFECT OF RETROFITTING ON FLEXURAL RIGIDITY OF RECTANGULAR FRP PLATES
EFFECT OF RETROFITTING ON FLEXURAL RIGIDITY OF RECTANGULAR FRP PLATES STEVEN J. MAKONIS, JR. Department of Civil & Environmental Engineering Old Dominion University Norfolk, VA 235280241, USA smako001@odu.edu
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationBondSlip Characteristics between ColdFormed Metal and Concrete
Missouri University of Science and Technology Scholars' Mine International Specialty Conference on Cold Formed Steel Structures (2014)  22nd International Specialty Conference on ColdFormed Steel Structures
More informationMacroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs
Macroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs JingZhong Xie 1 Abstract: The macroscopic Poisson ratio and elastic moduli of the castinplace hollowcore slab are researched
More informationMECE 3321: Mechanics of Solids Chapter 6
MECE 3321: Mechanics of Solids Chapter 6 Samantha Ramirez Beams Beams are long straight members that carry loads perpendicular to their longitudinal axis Beams are classified by the way they are supported
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationStrength Prediction Of Composite Laminate
Strength Prediction Of Composite te Prof. Yogananda. A 1, Mr. R. Vijayakumar 2 Assistant Professor, Department of Mechanical Engineering, East West Institute of Technology, Bangalore. Research Scholar,
More information2012 MECHANICS OF SOLIDS
R10 SET  1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~
More informationCalibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques
9 th International LSDYNA Users Conference Optimization Calibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques Stefano Magistrali*, Marco
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationBending Load & Calibration Module
Bending Load & Calibration Module Objectives After completing this module, students shall be able to: 1) Conduct laboratory work to validate beam bending stress equations. 2) Develop an understanding of
More informationPart 1 is to be completed without notes, beam tables or a calculator. DO NOT turn Part 2 over until you have completed and turned in Part 1.
NAME CM 3505 Fall 06 Test 2 Part 1 is to be completed without notes, beam tables or a calculator. Part 2 is to be completed after turning in Part 1. DO NOT turn Part 2 over until you have completed and
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationTESTING AND ANALYSIS OF COMPOSITE SKIN/STRINGER DEBONDING UNDER MULTIAXIAL LOADING.
TESTING AND ANALYSIS OF COMPOSITE SKIN/STRINGER DEBONDING UNDER MULTIAXIAL LOADING. Ronald Krueger*, Michael K. Cvitkovich*, T. Kevin O'Brien**, and Pierre J. Minguet*** * National Research Council Research
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationCHAPTER II EXPERIMENTAL INVESTIGATION
CHAPTER II EXPERIMENTAL INVESTIGATION 2.1 SCOPE OF TESTING The objective of this research is to determine the force distribution between the column web and stiffener when the column flanges are subjected
More informationNUMERICAL ANALYSIS OF SANDWICH PANELS SUBJECTED TO POINT LOADS
ECCOMAS Congress 216 VII European Congress on Computational Methods in Applied Sciences and Engineering M. Papadrakakis, V. Papadopoulos, G. Stefanou, V. Plevris (eds.) Crete Island, Greece, 5 1 June 216
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationSolid Mechanics Homework Answers
Name: Date: Solid Mechanics Homework nswers Please show all of your work, including which equations you are using, and circle your final answer. Be sure to include the units in your answers. 1. The yield
More informationAccelerated Testing Methodology for Long Term Durability of CFRP
IFREMERONR Workshop on Durability of Composites in a Marine Environment August 23 24, 22 IFREMER Centre, Nantes, France Accelerated esting Methodology for Long erm Durability of CFRP Masayuki Nakada*,
More informationACET 406 MidTerm Exam B
ACET 406 MidTerm Exam B SUBJECT: ACET 406, INSTRUCTOR: Dr Antonis Michael, DATE: 24/11/09 INSTRUCTIONS You are required to answer all of the following questions within the specified time (90 minutes).you
More informationUnit 18 Other Issues In Buckling/Structural Instability
Unit 18 Other Issues In Buckling/Structural Instability Readings: Rivello Timoshenko Jones 14.3, 14.5, 14.6, 14.7 (read these at least, others at your leisure ) Ch. 15, Ch. 16 Theory of Elastic Stability
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationFRACTURE MECHANICS APPROACHES STRENGTHENING USING FRP MATERIALS
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDIFICATIO Publishers, D79104 Freiburg, Germany FRACTURE MECHANICS APPROACHES STRENGTHENING USING FRP MATERIALS Triantafillou Department
More informationSolution: The moment of inertia for the crosssection is: ANS: ANS: Problem 15.6 The material of the beam in Problem
Problem 15.4 The beam consists of material with modulus of elasticity E 14x10 6 psi and is subjected to couples M 150, 000 in lb at its ends. (a) What is the resulting radius of curvature of the neutral
More informationDEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL
DEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL S. Quinn*, R.K. Fruehmann and J.M. DulieuBarton School of Engineering Sciences University of Southampton Southampton SO17
More informationMechanical Response of a Composite Steel, Concrete Filled Pile
Mechanical Response of a Composite Steel, Concrete Filled Pile Joseph Labuz, Principal Investigator Department of Civil, Environmental, and Geo Engineering University of Minnesota June 2018 Research
More informationSeismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design
Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design Elmer E. Marx, Alaska Department of Transportation and Public Facilities Michael Keever, California Department
More informationAmerican Society for Testing and Materials (ASTM) Standards. Mechanical Testing of Composites and their Constituents
Mechanical Testing of Composites and their Constituents American Society for Testing and Materials (ASTM) Standards Tests done to determine intrinsic material properties such as modulus and strength for
More informationNonlinear Modeling of FiberReinforced Elastomers and the Response of a Rubber Muscle Actuator
Nonlinear Modeling of FiberReinforced Elastomers and the Response of a Rubber Muscle Actuator Larry D. Peel, Ph.D.* Department of Mechanical & Industrial Engineering Texas A&M Univ.  Kingsville David
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More information3 A y 0.090
ROBLM.1 5.0 in. 5 8 in. diameter A standard tension test is used to determine the properties of an experimental plastic. The test specimen is a 5 in.diameter rod and it is subjected to an 800lb tensile
More information5. What is the moment of inertia about the x  x axis of the rectangular beam shown?
1 of 5 Continuing Education Course #274 What Every Engineer Should Know About Structures Part D  Bending Strength Of Materials NOTE: The following question was revised on 15 August 2018 1. The moment
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationPlease review the following statement: I certify that I have not given unauthorized aid nor have I received aid in the completion of this exam.
Group Number: Please review the following statement: I certify that I have not given unauthorized aid nor have I received aid in the completion of this exam. Signature: INSTRUCTIONS Begin each problem
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More information7 TRANSVERSE SHEAR transverse shear stress longitudinal shear stresses
7 TRANSVERSE SHEAR Before we develop a relationship that describes the shearstress distribution over the cross section of a beam, we will make some preliminary remarks regarding the way shear acts within
More informationThe numerical simulation research of an UltraLight Photovoltaic Cell multilayer composite structure
5th International Conference on Civil, Architectural and Hydraulic Engineering (ICCAHE 2016) The numerical simulation research of an UltraLight Photovoltaic Cell multilayer composite structure Kangwen
More informationand F NAME: ME rd Sample Final Exam PROBLEM 1 (25 points) Prob. 1 questions are all or nothing. PROBLEM 1A. (5 points)
ME 270 3 rd Sample inal Exam PROBLEM 1 (25 points) Prob. 1 questions are all or nothing. PROBLEM 1A. (5 points) IND: In your own words, please state Newton s Laws: 1 st Law = 2 nd Law = 3 rd Law = PROBLEM
More informationLecture 8 Viscoelasticity and Deformation
Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, µ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force to the strain in the direction of the applied force. For uniaxial
More informationEXPERIMENTAL AND NUMERICAL STUDY OF OBLIQUE IMPACT ON HELICOPTER BLADES INFLUENCE OF THE CURVATURE
EXPERIMENTAL AND NUMERICAL STUDY OF OBLIQUE IMPACT ON HELICOPTER BLADES INFLUENCE OF THE CURVATURE F. Pascal a, P. Navarro a*, S. Marguet a, J.F. Ferrero a, J. Aubry b, S. Lemaire b a Université de Toulouse,
More informationExperimental Behavior and DesignOriented Analysis of Sandwich Beams with. Biobased Composite Facings and Foam Cores
Experimental Behavior and DesignOriented Analysis of Sandwich Beams with Biobased Composite Facings and Foam Cores Dillon Betts 1 S.M.ASCE, Pedram Sadeghian 2 M.ASCE, and Amir Fam 3 F.ASCE ABSTRACT:
More informationtwenty one concrete construction: shear & deflection ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture twenty one concrete construction: Copyright Kirk Martini shear & deflection Concrete Shear 1 Shear in Concrete
More informationProblem d d d B C E D. 0.8d. Additional lecturebook examples 29 ME 323
Problem 9.1 Two beam segments, AC and CD, are connected together at C by a frictionless pin. Segment CD is cantilevered from a rigid support at D, and segment AC has a roller support at A. a) Determine
More informationME 354, MECHANICS OF MATERIALS LABORATORY COMPRESSION AND BUCKLING
ME 354, MECHANICS OF MATERIALS LABATY COMPRESSION AND BUCKLING PURPOSE 01 January 2000 / mgj The purpose of this exercise is to study the effects of end conditions, column length, and material properties
More informationNonlinear bending analysis of laminated composite stiffened plates
Nonlinear bending analysis of laminated composite stiffened plates * S.N.Patel 1) 1) Dept. of Civi Engineering, BITS Pilani, Pilani Campus, Pilani333031, (Raj), India 1) shuvendu@pilani.bitspilani.ac.in
More informationDYNAMIC ANALYSIS OF PILES IN SAND BASED ON SOILPILE INTERACTION
October 117,, Beijing, China DYNAMIC ANALYSIS OF PILES IN SAND BASED ON SOILPILE INTERACTION Mohammad M. Ahmadi 1 and Mahdi Ehsani 1 Assistant Professor, Dept. of Civil Engineering, Geotechnical Group,
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationSTUDY ON THE DAMAGE PROPAGATION OF A COMPOSITE SANDWICH PANEL WITH FOAM CORE AFTER LOW VELOCITY IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STUDY ON THE DAMAGE PROPAGATION OF A COMPOSITE SANDWICH PANEL WITH FOAM CORE AFTER LOW VELOCITY IMPACT Keywords: sandwich structures, foam, lowvelocity
More informationRailroad Concrete Tie Failure Analysis
Railroad Concrete Tie Failure Analysis Hailing Yu, David Jeong, Brian Marquis, and Michael Coltman 2014 International Crosstie & Fastening System Symposium June 35, 2014 The National Transportation Systems
More informationStress Transformation Equations: u = +135 (Fig. a) s x = 80 MPa s y = 0 t xy = 45 MPa. we obtain, cos u + t xy sin 2u. s x = s x + s y.
014 Pearson Education, Inc., Upper Saddle River, NJ. All rights reserved. This material is protected under all copyright laws as they currently 9 7. Determine the normal stress and shear stress acting
More informationMechanics of Materials II. Chapter III. A review of the fundamental formulation of stress, strain, and deflection
Mechanics of Materials II Chapter III A review of the fundamental formulation of stress, strain, and deflection Outline Introduction Assumtions and limitations Axial loading Torsion of circular shafts
More informationDiscrete Element Modelling of a Reinforced Concrete Structure
Discrete Element Modelling of a Reinforced Concrete Structure S. Hentz, L. Daudeville, F.V. Donzé Laboratoire Sols, Solides, Structures, Domaine Universitaire, BP 38041 Grenoble Cedex 9 France sebastian.hentz@inpg.fr
More information